**High-velocity instabilities in the vortex lattice of Nb/permalloy bilayers**

A. Angrisani Armenio,1C. Bell,2J. Aarts,2and C. Attanasio1

1_{Laboratorio Regionale SuperMat, CNR-INFM Salerno, and Dipartimento di Fisica “E. R. Caianiello,” Università degli Studi}*di Salerno, Baronissi, Salerno I-84081, Italy*

2_{Kamerlingh Onnes Laboratory, Leiden University, P.O. Box 9504, 2300 RA Leiden, The Netherlands}

共Received 13 April 2007; revised manuscript received 11 June 2007; published 1 August 2007兲
We have studied the critical current density*J _{c}*for onset of vortex motion and the dynamic instability of the
moving vortex lattice at high driving currents in superconducting共S兲/ferromagnetic共F兲Nb/ Ni

_{0.80}Fe

_{0.20}bilay-ers and in a single Nb film with the same thickness. The samples are all characterized by relatively high values of the pinning strength. The measured current-voltage characteristics are successfully described in the frame-work of the Larkin-Ovchinnikov model, modified in order to take into account the effect of the pinning close to the instability. We find that

*J*is smaller in the S/F bilayers than in the single film and argue that this is due to the strongly inhomogeneous order parameter in the bilayers. Also, the critical velocity

_{c}*v**

_{for the occurrence}of the instability is found to be significantly larger in the S/F bilayers than in the single S layer. By extracting the quasiparticle energy relaxation rate from

*v**

_{, we show that this effect is due to the same inhomogeneous}order parameter and the resulting lower average value of the superconducting gap.

DOI:10.1103/PhysRevB.76.054502 PACS number共s兲: 74.45.⫹c, 74.78.⫺w, 74.78.Fk

**I. INTRODUCTION**

The interplay between a superconductor 共S兲and a
ferro-magnet共F兲through the proximity effect in artificial S/F
hy-brids is currently a very active field of research involving
both fundamental and application aspects.1_{One of the }
pecu-liarities of S/F hybrids is the strongly inhomogeneous nature
of the superconducting order parameter. On the F side of the
interface, the interaction of the exchange field with the
Coo-per pairs causes the order parameter to oscillate,1,2 _{whereas}
on the S side, the order parameter is strongly suppressed over
a distance of the order of the superconducting coherence
length S, which is usually a few nanometers. The best
known consequences of this highly inhomogeneous character
of the order parameter are the strong suppression of the
su-perconducting critical temperature *Tc* with decreasing
S-layer thickness*dS*, and the nonmonotonic behavior of*Tc*as
function of the thickness*dF* of the F layer,3while in S/F/S
Josephson junctions, negative critical currents appear.4,5_{The}
nonhomogeneous character of the order parameter was also
recently studied by measuring the depairing current density

*Jdp*, which is determined by an average of the
superconduct-ing order parameter over the layer thickness.6,7

Such averaging should manifest itself also in other
prop-erties of the bilayer system. For instance, the force to pin
vortices in the superconductor can be expected to be
differ-ent, which is observable by measuring the onset of voltage at
the so-called critical current in the current 共*I*兲-voltage 共*V*兲

characteristic. Differences should also be found in behavior
of the moving vortex system. In particular, at high vortex
velocities, an instability can occur, which drives the system
to the normal state and therefore manifests itself by a jump in
the voltage. This instability, first described by Larkin and
Ovchinnikov共LO兲,8_{is related to the inelastic relaxation rate}
Eof quasiparticles inside the vortex core. Such instabilities
have been observed in a number of systems including
low-temperature9–12 _{and high-temperature superconducting}
thin films13–16_{and multilayers.}17–19_{What essentially emerges}

from these studies is that the voltage jumps are indeed due to
intrinsic properties of the moving vortex lattice but that two
more ingredients may play a role,共i兲the temperature
depen-dence ofE, in particular, when electron-electron interactions
dominate the relaxation, and 共ii兲 vortex pinning, ignored in
the original LO theory.20 _{The LO theory has been also }
ex-tended to explicitly consider the contributions due to the
heating effect.21_{Finally, measurements of flux-flow }
instabili-ties have been recently used to extract information about the
symmetry of the order parameter in YBa2Cu3O7 thin
films.22,23

In the present paper, we study LO instabilities in S/F
bi-layers of Nb/ Ni0.80Fe0.20, and for comparison in a single Nb
film, by measuring their*I*-*V* characteristics in perpendicular
magnetic fields. Using Ni_{0.80}Fe_{0.20} 共Permalloy兲, a strong
fer-romagnet, ensures that the order parameter is strongly
sup-pressed at the interface, so that the effects of the
inhomoge-neous order parameter can be investigated. The outline of the
paper is as follows. First, we give the theoretical framework
to describe and analyze the flux-flow instabilities, followed
by some experimental details. Results are then presented on
the critical current density*Jc*for the onset of vortex motion
and on the critical velocity *v** _{where the instability occurs.}
From the analysis of the instabilities as a function of the
temperature and magnetic field, we establish the role played
by the ferromagnet in determining the nonequilibrium Nb
properties.

**II. VORTEX LATTICE INSTABILITIES**

In the case of a vortex lattice moving under high applied
driving currents, Larkin and Ovchinnikov theoretically
pre-dicted a sudden voltage jump in the*I*-*V*curves before
reach-ing the value of the depairreach-ing current*Idp*.8 This fact is
im-portant not only from a fundamental point of view but it has
also practical implications because it establishes a limit for
the sustainable current in the superconducting state. The
abrupt switching of the sample to a state of higher electrical

resistance is caused by the electric field generated by the
vortex motion, which shifts the distribution of quasiparticles
inside the core to higher energies, causing some of them to
leave the core all together. The vortex core therefore shrinks
with increasing flux-line velocity*v*, and the viscous damping
coefficient decreases. For a critical value of the velocity*v**_{,}
the flux-flow state becomes unstable and the system switches
to the normal state. The amount of decrease of the damping
is controlled by the energy relaxation time of the
quasiparti-clesE. For the viscous damping coefficientas function of
the vortex velocity*v*, LO obtained the expression

共*v*兲=共0兲 1

1 +共*v*/*v**_{兲}2, 共1兲

where共0兲is the viscous damping coefficient at zero
veloc-ity. From Eq.共1兲, one sees that the damping force *Fv*=*v*
increases with increasing velocity until it reaches a
maxi-mum at *v*=*v**. Since *v* is proportional to the voltage *V*

through the Lorentz force, the current-voltage characteristics are, according to LO, described by the relation

*V*

1 +共*V*/*V**兲2+*cV*共1 −*t*兲

1/2_{=}_{共}_{I}_{−}_{I}

*c*兲*Rf f*, 共2兲

where*t*=*T*/*Tc* is the reduced temperature, *Ic* is the critical
current,*Rf f* is the flux-flow resistance, and*c*is a constant of
the order of unity. The curve starts to bend upward in the
vicinity of the critical voltage*V**_{, which is related to}* _{v}**

_{by}means of the relation

*V**=0*v***HL*, 共3兲

where*H*is the applied magnetic field and *L* is the distance
between the voltage contacts.

For the critical velocity LO found

*v**= *D*

1/2_{关14}_{}_{共3兲兴}1/4_{共1 −}_{t}_{兲}1/4

共E兲1/2 , 共4兲

where共*x*兲is the Riemann zeta function and*D*is the
*quasi-particle*diffusion coefficient, which means that from
measur-ing the critical voltage*V**_{it is possible to estimate values for}
E. As can be expected, faster relaxation共smallerE兲leads to
larger*v**_{. In this respect, it is important to note that a }
tem-perature dependence can also be expected forE. If the
domi-nant relaxation mechanism is electron-phonon scattering, it
should be E⬀*T*−3_{, while if electron-electron interactions}
dominate, it isE=E_{,}*el*exp关2⌬共*T*兲/*kBT*兴, whereE,*el*is
basi-cally the inelastic relaxation time of the electron system, and
⌬共*T*兲 has the temperature dependence ⌬共*T*兲=⌬共0兲共1
−*T*/*Tc*兲1/2 from the BCS theory. This exponential behavior
for E was indeed found in various materials, with ⌬共0兲
= 1.76*kBTc* as expected from the BCS theory for low-*Tc*
amorphous Mo3Si and ⌬共0兲= 3.5*kBTc* for high-*Tc*
YBa2Cu3O7 共Ref.14兲 in accordance with the enhanced gap
values in high-*Tc* materials. In Ta/ Ge multilayers, again
⌬共0兲= 1.76*kBTc* was found when the Ta layers were
un-coupled, while a coupled anisotropic multilayer yielded
⌬共0兲= 3.5*kBTc*,18 indicating that the anisotropy leads to an

*effective* value for ⌬共0兲 without changing the exponential
dependence.

Another point to note is that in the LO theory, the critical
velocity 关Eq. 共4兲兴 should not be dependent on the external
magnetic field.8_{However, it was discussed that the LO }
con-dition for a spatially homogeneous quasiparticle
nonequilib-rium distribution is only met when the distance*v**_{E}_{is larger}
than the intervortex distance*a*_{0}. At low magnetic fields, this
is not the case, and*v**becomes proportional to*a*0and
there-fore to

### 冑

1 /*H*.14

_{The crossover between the two regimes takes}place when

*v**E=*a*0*f*共*T*兲, 共5兲
where*f*共*T*兲 is a numerical factor of the order of unity.

**III. EXPERIMENT**

A Nb film and Nb/Py bilayers were prepared by dc sputter
deposition on oxidized Si共100兲 substrates in an ultrahigh
vacuum system.24_{We studied one single 25 nm thick Nb film}
and two bilayers with the same Nb thickness*d*Nb= 25 nm and
Py thickness *d*Py= 10 and 75 nm, respectively. As we will
see, in all samples, the pinning is relatively high, with the
low-field critical current density values higher than
109A / m2 at *t*=*T*/*Tc*= 0.5. Py, apart from having a quite
large spin polarization25 _{is characterized by very small }
val-ues of the coercive fields *Hc* at low temperatures, slightly
dependent on thickness. Typical values for *Hc* in our
samples, measured with an in-plane field, are around 2 mT

共10 mT兲 for 50 nm共20 nm兲 thick Py films.26 The low

coer-civity, the preferential in-plane magnetization, and the very small thickness make that domain configurations or flux variations in the superconductor due to the ferromagnet do not play a role in our experiments, which are carried out in perpendicular applied field. Even a small in-plane field, for instance, due to external stray fields or a small misalignment of the sample normal with respect to the applied field, will drive out the domains and make the in-plane magnetization uniform. The large demagnetization factor then ascertains that the amount of flux produced by the small volume of the ferromagnetic layer is negligible; in other words, the mag-netic induction equals the applied field.

the temperature dependence of the perpendicular upper
criti-cal magnetic fields*Hc*2⬜共*T*兲were resistively measured in the
four contact configuration; the values were extracted from
the *R*共*T*兲 curves, taking the 90% value of the normal state
resistance*RN*just above the transition to the superconducting
state. The transition widths, estimated from the temperature
difference at 10% and 90% of *RN*, were typically less than
60 mK at zero field and did not substantially broaden, even
in high perpendicular magnetic fields, confirming the high
quality of our samples. From the slope of the perpendicular
upper critical field,27 _{it is also possible to estimate}
the quasiparticle diffusion coefficient *D*=共4*kB*/*e*兲
⫻共−*dHc*2⬜/兩*dT*兩*T*=*T _{c}*兲−1for the single Nb film. Because in
lay-ered S/F systems the

*Hc*2⬜共

*T*兲 curves shift in a parallel way as a function of the layer thicknesses, the slope of the per-pendicular upper critical field cannot be used directly to de-termine

*D*for the two Nb/Py bilayers.28,29

_{We will take}

_{D}_{for}Nb for all the calculations. Some characteristic parameters of the measured samples are reported in Table I. Note that

*Tc*for the bilayers has decreased by about 1.5 K, which means that the order parameter, assumed to be close to zero at the interface, has relaxed substantially to the bulk value. We therefore expect it to be inhomogeneous over the full film thickness.

**IV. RESULTS AND DISCUSSION**

**A. Critical currents**

In Fig. 1共a兲, the *I*-*V* characteristics are shown for the
single Nb film at*t*= 0.5 for different values of the external
magnetic field between 0.05 and 1.8 T as indicated. Up to a
certain value of the magnetic field, the curves exhibit a
sud-den jump at a well defined current value*I**, well above the
critical current *Ic* where the onset of voltage occurs. At
higher magnetic fields, the*I*-*V*curves become more smeared
and finally the jump disappears. This observation is
consis-tent with other results found on different kinds of

supercon-ducting systems.9–19 _{Very similar behavior is observed for}
both Nb/Py bilayers. In Fig.1共b兲, we show the *I*-*V* curves,
also measured at*t*= 0.5, for the NbPy75 sample.

The critical current density *Jc*=*Ic*/共*wd*兲 共*d* is the sample
thickness兲 at*t*= 0.5 for the three samples is shown in Fig.2
as a function of the external magnetic field. The critical
cur-rent*Ic*was defined using a dc voltage criterion of 2V. For
all samples,*Jc*rises quickly when the field is lowered below

*Hc*2 and becomes more or less constant below *Hc*2/ 2. At
these low fields, where the pinning is individual rather than
collective, the values for*Jc*range from 109A / m2for NbPy75
to 5⫻1010_{A / m}2 _{for Nb. The pinning is therefore quite}
strong in comparison, for instance, with amorphous
materi-als. Also, the values for the two Nb/Py bilayers are
substan-tially smaller than for the single film and we want to argue
that this is an immediate consequence of the *homogeneous*

TABLE I. Characteristic parameters of the measured samples.
*d*_{Nb}共*d*_{Py}兲is the Nb共Py兲layer thickness,*T _{c}*is the critical
tempera-ture,

*n*is the normal state resistivity measured at

*T*= 10 K,

*H _{c}*

_{2}

_{⬜}共

*t= 0.5*兲 is the value of the perpendicular critical field at the reduced temperature equal to 0.5, and

*D*is the quasiparticle diffu-sion coefficient as determined from the

*Hc*2⬜ versus temperature

curve for the single Nb film.

Sample

*d*Nb

共nm兲

*d*Py

共nm兲

*Tc*
共K兲

Nb 25 0 8.59

NbPy10 25 10 6.97

NbPy75 25 75 6.72

*n*
共⍀cm兲

*H _{c}*

_{2}

_{⬜}

共*t= 0.5*兲共*T*兲

*D*

共m2/ s兲

Nb 7.4 1.75 2.78⫻10−4

NbPy10 2.4 0.75

NbPy75 6.7 0.75

suppression of the order parameter inside the Nb. The
single-vortex pinning in superconducting films is due to defects in
the crystal lattice which can be pointlike or extended共grain
boundaries兲 and which cause local variations in the order
parameter. Such defects pin vortices because of the smaller
amount of condensation energy which locally has to be paid
when the vortex resides there. In the region of
homoge-neously suppressed superconductivity, which is basically the
whole film, the local energy gain is less, and the pinning
consequently weaker. We want to note that this is opposite to
what can be expected for a magnetic impurity in the
super-conducting matrix. In that case, the local suppression is
stronger than that of ordinary defects and the pinning will be
stronger, as was indeed found in NbTi wires with Ni and Fe
impurities.30 _{The effect is also opposite to the effect from}
domain walls in the ferromagnet which can pin a vortex by
its flux.31,32

Although not central to the paper, we can also remark that
the relatively strong pinning in all samples appears to
deter-mine the precise shape of the*I*-*V* curves. Equation共2兲, for

*I*⬎*Ic*, describes the *I*-*V* curves close to the instability only
when pinning mechanisms are absent and in high enough
fields that the flux-flow resistance*f*is given by the
Bardeen-Stephen limitf=n*H*/*Hc*2, withnthe normal state
resistiv-ity. To include the effect of low fields and pinning, the*I*-*V*

relation should be modified as follows18_{:}

*I*= *V*

*Rn*

## 冋

␣共1 +*V*−*c*兲

1 +共*V*/*V**兲2 + 1

## 册

, 共6兲where␣, , and *c* are constants and used as fitting
param-eters. The constant␣corrects for the low-field flux-flow
re-sistance; the other two constants parametrize the correction
to the viscosity constant by the pinning. In Figs. 3共a兲 and
3共b兲, we show the initial part of the*I*-*V* curves close to the
instability, for the Nb film and for the NbPy75 bilayer,
re-spectively. The solid lines are the fits to the experimental
points obtained by using Eq.共6兲. The fits are good, and the
values obtained for the parameter␣are quite small共around
10 or less兲for all the magnetic fields in agreement with the

results reported for high-pinning multilayers.18_{Also, with the}
obtained values for␣,, and*c*, the theoretical curves do not
show any back bending which results in hysteresis not due to
thermal origin in the*I*-*V*characteristics.10,18_{Such hysteresis}
has been observed on amorphous Mo3Si for which, however,
the estimated value for the parameter␣ was equal to 14.10

**B. Critical velocities**

Next, we come to the analysis of the critical velocities.
We interpret the voltage*V**corresponding to the value of the
current*I**, where the jumps in the*I*-*V*curves appear, as the
LO flux-flow instability at the velocity*v**_{. The values of}* _{v}**

_{,}as obtained directly from the measured

*V**

_{using Eq.}

_{共}

_{3}

_{兲}

_{, are}plotted as a function of

*H*for the single Nb film and for the two Nb/Py bilayers in Figs.4共a兲and4共b兲, respectively. In the insets, the behavior of

*v**

_{versus}

*−1/2*

_{H}_{at}

_{t}_{= 0.5 for the three}FIG. 2. Critical current density versus perpendicular magnetic

field at*t= 0.5 for the three analyzed samples.*

samples is shown. In both cases, the data in low fields show
the critical velocity to be proportional to *H*−1/2, indicating
that thermal effects are not responsible for the observed
in-stability. For the Nb film, also the crossover to a
field-independent*v**_{is found. For the Nb/Py bilayers, the }
instabil-ity disappears already at field around 0.15 T, and we cannot
detect the crossover. The numbers show that the critical
ve-locities in the case of the Nb/Py bilayers are much larger and
the instability disappears in this case already at smaller fields
because the critical voltage*V**is always much closer to *VN*

共the normal state voltage兲 with respect to what happens in

the single Nb film. Also, no substantial difference appears in
the results obtained on the two Nb/Py bilayers. This is
prob-ably not surprising since Py is characterized by an induced
superconducting coherence length of the order of only
1 nm.33_{However, as noticed in the literature,}12,18,21_{the}* _{H}*−1/2
dependence of

*v**

_{can also be induced by unavoidable Joule}heating. In this case, a well defined theoretical expression is predicted for the dissipated power

*P**

_{=}

***

_{I}***

_{V}_{as a function of}

*H*/*HT*.12,15,21Here,*I**is the current value where instabilities
take place and *HT* is a characteristic magnetic field where

thermal effects start to strongly influence the flux-flow
insta-bilities. We did not find any agreement between theory and
experiment for the Nb film, while in the case of both the
Nb/Py samples, we get_{0}*HT*= 0.20 T, implying that thermal
heating does not considerably influence the field dependence
of the measured critical velocities.

What we believe to be the central point of our
measure-ments is the fact that for the two Nb/Py bilayers, the *v**
values are much larger than for the Nb single film. Looking
at Eq. 共4兲, this must reflect in very different values for the
relaxation time E for the two systems. In Fig. 5, the
tem-perature dependenceE is given of for the single Nb film at
two different fields, _{0}*H*= 0.45 T above and _{0}*H*= 0.20 T
below the crossover field to constant*v** _{at}_{t}_{= 0.5. The solid}
lines are the curvesE=E,*el*exp关*m*⌬共*T*兲/*kBT*兴 withE,*el*and

*m* both used as fitting parameters. We obtain E,*el*= 9.74
⫻10−11_{s and} _{m}_{= 1.9 for} _{}

0*H*= 0.45 T and E,*el*= 6.68
⫻10−12_{s and}_{m}_{= 1.8 for}_{}

0*H*= 0.20 T. The dashed lines are
the fit to the experimental data using the expression E
⬀*T*−*n*, where for both fields we obtain the unphysical value

*n*= 9 for the exponent. The result tells us that
electron-electron scattering dominates the energy relaxation in Nb
film and that the temperature dependence is due to that of the
gap, with⌬共0兲⬇1.76*kBTc*as expected from the BCS theory.
Moreover, the values for E,*el*are the right order of
magni-tude. Similar findings are obtained for the temperature
de-pendence of E in the two Nb/Py bilayers. Figure. 5 also
shows the temperature dependence of E for the sample
NbPy10 at _{0}*H*= 0.15 T. The dashed line refers to the
power-law fit to experimental data with*n*= 5, again
unphysi-cal, and the solid line is the exponential fit. In this case,
E,*el*= 2.80⫻10−12s, not very different from the number for
the Nb film in 0.2 T. The coefficient*m*, however, turns out to
be equal to 1.0, suggesting that the effective gap experienced
by the quasiparticles in their relaxation process is only half
of the bulk gap. The much larger共critical兲velocities for
vor-tices in the bilayer system therefore appear directly related to
FIG. 4. Critical velocity *v**_{versus applied magnetic field at} _{t}

= 0.5共a兲for Nb film and共b兲for the two Nb/Py bilayers. Insets:*v**
versus *H*−1/2_{at}_{t}_{= 0.5}_{共}_{a}_{兲} _{for Nb film and} _{共}_{b}_{兲} _{for the two Nb/Py}
bilayers. The solid lines are guides to the eyes to show the*H*−1/2
proportionality of*v**.

FIG. 5. *E* temperature dependence for the Nb single film at

0*H= 0.45 T and* 0*H= 0.20 T and for NbPy10 at* 0*H= 0.15 T.*
The dashed lines are the fit to the experimental data using the
ex-pression *E*⬀*T*−*n*, while the solid lines are the fitting curves

the suppression of the superconducting order parameter in the S layer.

**V. CONCLUSIONS**

We have studied the *I*-*V* characteristics at different
per-pendicular magnetic fields and temperatures for a Nb single
film and for two Nb/Py bilayers with different Py
thick-nesses. Critical currents in Nb/Py samples are much smaller
than those measured in the single Nb film. We have also
observed sudden jumps in the*I*-*V*curves due to an instability
of the vortex lattice which could not be ascribed to heating

effects of the samples. The values of the critical velocities connected to the measured instabilities are much larger in Nb/Py with respect to the Nb. The above experimental find-ings are consistently interpreted as an effect of the strong inhomogeneity of the order parameter in the Nb layer when in contact with the ferromagnet.

**ACKNOWLEDGMENT**

This work is part of the research program of the “Stich-ting voor Fundamenteel Onderzoek der Materie 共FOM兲,” which is financially supported by the “Nederlandse Organi-satie voor Wetenschappelijk Onderzoek共NWO兲.”

1_{A. I. Buzdin, Rev. Mod. Phys.} _{77}_{, 935}_{共}_{2005}_{兲}_{.}

2_{E. A. Demler, G. B. Arnold, and M. R. Beasley, Phys. Rev. B} _{55}_{,}
15174共1997兲.

3_{I. A. Garifullin, J. Magn. Magn. Mater.} _{240}_{, 571}_{共}_{2002}_{兲}_{.}
4_{V. V. Ryazanov, V. A. Oboznov, A. Yu. Rusanov, A. V. }

Vereten-nikov, A. A. Golubov, and J. Aarts, Phys. Rev. Lett. **86**, 2427

共2001兲.

5_{T. Kontos, M. Aprili, J. Lesueur, F. Genet, B. Stephanidis, and R.}
Boursier, Phys. Rev. Lett. **89**, 137007共2002兲.

6_{C. Cirillo, A. Rusanov, C. Bell, and J. Aarts, Phys. Rev. B} _{75}_{,}
174510共2007兲.

7_{J. M. E. Geers, M. B. S. Hesselberth, J. Aarts, and A. A. Golubov,}
Phys. Rev. B **64**, 094506共2001兲.

8_{A. I. Larkin and Yu. N. Ovchinnikov, Sov. Phys. JETP} _{41}_{, 960}

共1976兲.

9_{W. Klein, R. P. Huebener, S. Gauss, and J. Parisi, J. Low Temp.}
Phys. **61**, 413共1985兲.

10_{A. V. Samoilov, M. Konczykowski, N.-C. Yeh, S. Berry, and C.}
C. Tsuei, Phys. Rev. Lett. **75**, 4118共1995兲.

11_{C. Villard, C. Peroz, and A. Sulpice, J. Low Temp. Phys.} _{131}_{,}
957共2003兲.

12_{C. Peroz and C. Villard, Phys. Rev. B} _{72}_{, 014515}_{共}_{2005}_{兲}_{.}
13_{S. G. Doettinger, R. P. Huebener, R. Gerdemann, A. Kühle, S.}

Anders, T. G. Träuble, and J. C. Villegier, Phys. Rev. Lett. **73**,
1691共1994兲.

14_{S. G. Doettinger, S. Kittelberger, R. P. Huebener, and C. C. Tsuei,}
Phys. Rev. B **56**, 14157共1997兲.

15_{Z. L. Xiao, P. Voss-de Haan, G. Jakob, and H. Adrian, Phys. Rev.}
B **57**, R736共1998兲.

16_{Z. L. Xiao, P. Voss-de Haan, G. Jakob, Th. Kluge, P. Haibach, H.}
Adrian, and E. Y. Andrei, Phys. Rev. B **59**, 1481共1999兲.
17_{B. J. Ruck, J. C. Abele, H. J. Trodahl, S. A. Brown, and P. Lynam,}

Phys. Rev. Lett. **78**, 3378共1997兲.

18_{B. J. Ruck, H. J. Trodahl, J. C. Abele, and M. J. Geselbracht,}
Phys. Rev. B **62**, 12468共2000兲.

19_{C. Peroz, C. Villard, A. Sulpice, and P. Butaud, Physica C} _{}**222-226**, 369共2002兲.

20_{Z. L. Xiao and P. Ziemann, Phys. Rev. B} _{53}_{, 15265}_{共}_{1996}_{兲}_{.}
21_{A. I. Bezuglyj and V. A. Shklovskij, Physica C} _{202}_{, 234}_{共}_{1992}_{兲}_{.}
22_{B. Kalisky, Y. Wolfus, Y. Yeshurun, G. Koren, and R. P. }

Hue-bener, Physica C **401**, 273共2004兲.

23_{B. Kalisky, P. Aronov, G. Koren, A. Shaulov, Y. Yeshurun, and R.}
P. Huebener, Phys. Rev. Lett. **97**, 067003共2006兲.

24_{A. Yu. Rusanov, M. Hesselberth, J. Aarts, and A. I. Buzdin, Phys.}
Rev. Lett. **93**, 057002共2004兲.

25_{J. S. Moodera, J. Nowak, and R. J. M. van de Veerdonk, Phys.}
Rev. Lett. **80**, 2941共1998兲.

26_{A. Yu. Rusanov S. Habraken, and J. Aarts, Phys. Rev. B} _{73}_{,}
060505共R兲 共2006兲.

27_{J. Guimpel, M. E. de la Cruz, F. de la Cruz, H. J. Fink, O. }
La-borde, and J. C. Villegier, J. Low Temp. Phys. **63**, 151共1986兲.
28_{Z. Radovic, L. Dobrosavljevic-Grujic, A. I. Buzdin, and J. R.}

Clem, Phys. Rev. B **38**, 2388共1988兲.

29_{P. Koorevaar, Y. Suzuki, R. Coehoorn, and J. Aarts, Phys. Rev. B}
**49**, 441共1994兲.

30_{N. D. Rizzo, J. Q. Wang, D. E. Prober, L. R. Motowidlo, and B.}
A. Zeitlin, Appl. Phys. Lett. **69**, 2285共1996兲.

31_{L. N. Bulaevskii, E. M. Chudnovsky, and M. P. Maley, Appl.}
Phys. Lett. **76**, 2594共2000兲.

32_{M. Z. Cieplak, X. M. Cheng, C. L. Chien, and H. Sang, J. Appl.}
Phys. **97**, 026105共2005兲.